# Dots - arxiv.org

Embed Size (px)

### Transcript of Dots - arxiv.org

The Emission Directionality of Electronic Intraband Transitions in Stacked QuantumDots

Alexander Mittelstadt,∗ Ludwig A. Th. Greif, and Andrei SchliwaInstitut fur Festkorperphysik, Technische Universitat Berlin,

Hardenbergstr. 36, 10623 Berlin, Germany(Dated: August 20, 2021)

We investigate the emission directionality of electronic intraband (intersubband) transitions instacked coupled quantum dots. Using a well-established eight-band k · p method, we demonstratethat the minor contributions from the valence band mixing into the conduction band govern thepolarization and emission directionality of electronic p-to-s-type intraband transitions. Despite thatthe contribution from the central-cell part to the momentum matrix element is dominant, we find,the contribution from the matrix elements among the envelope functions cannot be neglected. Withthe help of an artificial cuboidal quantum dot, we show that the vertical emission from intrabandtransitions can be tuned via the emitter’s vertical aspect ratio. Subsequently, we show that theseresults can be transferred to more realistic geometries of quantum dots and quantum dot stacksand demonstrate that the vertical emission can be enhanced from 23 % to 46 % by increasing theemitter’s vertical aspect ratio to the isotropic case with a vertical aspect ratio of 1.0. Therefore, astacking of a few quantum dotss (∼4 for the investigated structures) is already sufficient to improvethe vertical radiation significantly. Additionally, we discuss the impact of the number of stackedQDs as well as the effect of the interdot coupling strength on the radiation properties.

I. INTRODUCTION

Compact semiconductor light emitters and detectorsoperating within the infrared spectrum gained interestwithin last years as terahertz devices provide the highfrequencies needed, e.g., for next generation wireless com-munications systems; see Refs. [1–5]. Widely tunable in-traband (intersubband) transitions in quantum dot (QD)heterostructures can play a crucial role in the develop-ment of suitable infrared devices, whereas QD semicon-ductor devices also show high temperature stability andnarrow linewidths; cf. [6–9]. In addition, since infraredintraband transitions in quantum well devices are for-bidden for light polarized perpendicular to the growthdirection (normal incident light), QD-based systems arebetter suited for infrared sensors (IR photo detectors)[10–15], low-threshold terahertz vertical-cavity surface-emitting lasers [16, 17], and photovoltaic [18–21].In contrast to the polarization of interband transitions insingle and stacked QDs (see, e.g., Refs. [22–31]), a com-prehensive study of the polarization and emission proper-ties of intraband transitions of QD stacks is still missing.Studies on single QDs and stacks of two QDs (forminga QD molecule) show that electronic intraband transi-tions in QDs exhibit a fundamentally different spatialemission as interband transitions [32–37]. As well, Sheng[35] found that the polarization of intraband transitionscan be explained by the symmetry of valence band func-tions, in other words, by directed interactions of the lo-cal atomic orbitals. It was also found that the mixing ofthese valence band functions into the conduction bandstates is different for a QD molecule compared to a sin-gle QD, giving rise to other transition matrix elements

[34]. Based on these preliminary findings on transitionmatrix elements, we show a comprehensive study of theradiation properties of stacked QDs, guiding the designand growth of such QD structures, potentially makinginfrared devices more efficient. Although polarization-resolved transition matrix elements can be derived anal-ogous to interband transitions [30, 31, 38–42], which inturn can be used to calculate angle-resolved radiationintensities [22], studies investigating the emission direc-tionality of intraband transitions of QD stacks are stilllacking. In this article, we focus on the vertical aspectratio (AR) of the emitter as we found that the emitter’sconfinement region’s aspect ratio has a decisive impact onthe emission direction of the intraband transitions sim-ilar to that of the interband transitions. By stackingQDs, ensembles of 30 and more vertically coupled QDscan be formed, changing the emitter’s AR and where theinterdot coupling strength is adjusted via the separatingbarrier width [24, 43, 44].This article is organized as follows: First, we outline themethod of calculating the QDs electronic structure andthe determination of the radiation pattern of CB intra-band transitions. Next, we examine three different se-ries of QDs and highlight the effect of changing the QDstack’s morphology on its radiation pattern. Series Aconsists of artificial cubodial QDs, which help to iden-tify the impact of the QDs AR on emission propertiesof stacked QDs; see Fig. 1(a). Series B and C are usedto compare our findings with series A with more realisticQD structures: Here, stacks of InGaAs/GaAs QDs are in-vestigated, mapping the most basic parameters changingthe AR of the spatial confinement and the QDs couplingstrength, showing that the findings from Series A can betransferred to realistic structures. In Series B, we demon-strate the impact of the number of QDs stacked. Here,for closely stacked QDs, the stack number is varied from

arX

iv:2

108.

0876

1v1

[co

nd-m

at.m

es-h

all]

19

Aug

202

1

2

1/2 2

A

B

C

1/2

1 (b)(a)

radial distance in hQDIn

dium

cont

ent

Figure 1. (a) The QD structures investigated. Series A:nine artificial cubodial QDs with AR between 1.6 and 0.4.Series B: stacks of ten identical QDs to a single QD withbarrier width of b = 0 monolayers (MLs). Series C: stacksof nine identical QDs with barriers varying from b = 0 MLsto b = 16 MLs. (b) Scheme of the modeled QD geometrywith a gradual composition. The Indium x content withinan InxGa1−xAs QD as a function of the distance to the apexcenter in units of the QD’s height hQD.

a single QD to a stack of ten QDs. For series C, for astack of five QDs, the interdot distance and thus the QDcoupling strength is changed from closely stacked intoa weak coupling regime until the QDs decouple. For se-ries B and C, InxGa1−xAs QDs are modeled as truncatedpyramids with a side-wall inclination of 40, embedded ina GaAs matrix, in agreement with investigations in Refs.[45, 46]. The model QDs have a base diameter of 17.5 nmand a height of 3.4 nm, in agreement with experimentalinvestigations of stacked InAs QDs [28, 43, 47, 48]. Theindium content decreases linearly (see Fig. 1(b)) in agree-ment with experimental investigations and findings thatuniform compositions are not able to reproduce the cor-rect electron-hole alignment and polarization propertiesfor interband transitions [49–54].

II. METHOD OF CALCULATION

Calculations of the emission directionality of intrabandCB transitions in stacks of up to ten QDs are build onan established 8-band k · p model; see Refs. [33, 55, 56].By using the k ·p model, electronic structure calculationsof extended QD systems are more efficient compared toatomistic models. Furthermore, long-range interactionslike strain and strain-induced piezoelectricity are consid-ered, which usually have to be omitted by atomistic the-ories; cf. Refs. [57–60] and references therein. In theeffective mass approximation, single-particle states arerepresented as a product basis

|ψ〉 =

8∑k=1

|φk〉 |uk〉 , (1)

with the envelope |φk〉 and the atomic-like bandedge (Γ-point) Bloch functions

|u〉 = [|s ↑〉 , |x ↑〉 , |y ↑〉 , |z ↑〉 , |s ↓〉 , |x ↓〉 , |y ↓〉 , |z ↓〉]T ,(2)

where the arrows denote the spin and the |s〉, |x〉 , |y〉 , |z〉denote the s- and p-type bandedge Bloch functions, re-spectively. It is also possible to transform the Bloch ba-sis into another set of eigenfunctions of the Hamiltonian,which represent the states in a conduction (CB) and va-lence band (VB) Bloch basis; see Refs. [61–63]. For ex-ample, considering quantization along the z-axis,

|cb1〉|hh1〉|lh1〉|so1〉

...

=

i |s ↓〉|x〉+i|y〉√

2|↑〉

|x〉−i|y〉√6|↑〉+ 2|z〉√

6|↓〉

|x〉−i|y〉√3|↑〉 − |z〉√

3|↓〉

...

, (3)

where the dots represent the functions |cb2〉, |hh2〉, |lh2〉,and |so2〉 build from bandedge Bloch functions with op-posite spin in Eq. 2 and |cb1〉 = |ucb ↓〉, and so on. Here,the |cb〉 denote the CB and the |hh〉, |lh〉, and |so〉 theheavy, light, and splitoff VB states, respectively. In gen-eral, any state |ψ〉 can be represented in this basis set byprojection onto the respective basis functions

| 〈uk|ψ〉 |2 = | |φk〉 |2 . (4)

The lattice mismatch of InAs and GaAs (about 7%) re-sults in a highly strained heterostructure shifting the CBvia the deformation potentials ac, av, and b; cf. Refs.[63, 64]. The simplified equation in Ref. [63] illustratesthe strain-induced band coupling for the CB

VCB = ECB + aceh (5)

and the VB VVB = EVB + aveh ± b2eb, where ECB and

EVB are the unstrained CB edges, respectively. The ehand eb are the hydrostatic and biaxial strain components,respectively. Thus, the hydrostatic strain is shifting theCB’s energetic position, while in contrast, the VB is alsoinfluenced by the biaxial strain resulting in a splitting ofthe light- and heavy-hole band. Consequently, the con-finement region and the strain determine the characterof the hole ground state, i.e., the leading |hh〉 and |lh〉contributions, respectively, which have a decisive influ-ence on the polarization of the electron-hole decay [22].In contrast to the hole ground state, the lowest CB stateis less affected by the strain (see Ref. [62]) and the enve-lope’s symmetry is not changed. The leading contribu-tions of the CB states is, at least for the InGaAs/GaAsQD systems considered, always s-like, but the VB statesmix into the states and influence the polarization of theCB intraband transitions and thus their radiation char-acteristics; cf. Refs. [34, 35, 63]. Similar to the change

3

of the VB groundtate’s composition considered for inter-band transitions (see Ref. [22]), the |hh〉 and |lh〉 contri-bution of the CB groundstate change for stacks of QDswith different heights and spacings. This is particularlyrelevant as enlarged |hh〉 or |lh〉 contributions result inenhanced horizontal or vertical plus horizontal polariza-tion of the intraband transitions, respectively, owing tothe different components from the bandedge Bloch func-tions; cf. Eq. 3.In Fermi’s golden rule, the matrix element for a transi-tion between state |i〉 and state |j〉 using the expansionin Eq. 1 is

〈j|ε · p|i〉 =∑kl=1

δkl 〈φjk|ε · p|φil〉︸ ︷︷ ︸(a)

+∑kl=1

〈φjk|φil〉 〈ujk|ε · p|uil〉︸ ︷︷ ︸(b)

, (6)

where |j〉 = |ψj〉. While interband transitions aregoverned by the second term (b) and are calculatedvia the optical matrix elements of the bandedge Blochfunctions, considering intraband transitions non of bothterms might be neglected, whereby the matrix element(a) is calculated from the envelope functions involved,i.e., 〈ujk|uil〉 = 1. The emission rate is

Γi,j(ε) ∝∣∣∣[(a) + (b)]

∣∣∣2 . (7)

We derive the rate of emitted photons Γi,j as a func-tion of their polarization ε(φε, θε) and their propagationdirection k(φk, θk) by assuming a transversal propaga-tion. Using a frame of reference ρ, ϕ, ϑ (in spherical co-ordinates), with the z′-axis aligned to the propagationdirection k, the integrated transition rate for all possi-ble polarizations can be written as a line integral in theϑ = π/2-plane

Γi,j(k) =∑o

[ ∫ 2π

0

dϕΓi,j(ϕ, π/2)]. (8)

Here, o is the sum over all degenerate intraband states |ψ〉considered for the transition. Throughout this article, weuse a spatially resolved emission intensity parametrizedin the QD’s frame of reference using the condition ε ·k =0. Equation 8 simplifies to

Γi,j(k) =∑o

[ ∫ε⊥k

dΩQDε Γi,j(ε)

], (9)

where φk and θk define the propagation direction. If therate Γi,j(k) is calculated, each transition is counted sev-eral times, thus, the rate is normalized to the total rateof emitted photons. We calculate the degree of radiationanisotropy (DORA) for the three perpendicular crystalplanes. Here, we use, analogously to the degree of po-larization defined in Refs. [23, 24, 30, 41], the (110)- and

0.511.5

4

6

8

10

vertical aspect ratio

composition[%

]

no strainx,y z(b)

Figure 2. (a) Decomposition of the lowest conduction bandstate of the cubodial QD series A into the |cb〉 (blue circles),|hh〉 (green empty square), |lh〉 (green filled square), and |so〉(red pyramid) basis functions versus vertical aspect ratio. (b)Corresponding decomposition into the atomic-like basis func-tions |x〉, |y〉 (blue pyramid), and |z〉 (red inverted pyramid).Both diagrams are calculated excluding effects of strain.

(110)-plane as an indicator for the degree of the QD sys-tems top- and in-plane-emission:

DORA(001) =Γ(k = [110])− Γ(k = [110])

Γ(k = [110]) + Γ(k = [110])(10)

DORA(110) =Γ(k = [110])− Γ(k = [001])

Γ(k = [110]) + Γ(k = [001])(11)

DORA(110) =Γ(k = [110])− Γ(k = [001])

Γ(k = [110]) + Γ(k = [001])(12)

III. DISCUSSION AND RESULTS

As discussed above, interband transitions are governedby the central-cell term Eq. 6(b). If we now assumethat intraband transitions to be governed by Eq. 6(a),the trivial conclusion would be that CB px,y-to-s-type,| |ψs〉 |2 and | |ψpx,y

〉 |2, respectively, transitions absorb oremit light polarized within the (001)-plane. However,previous numerical investigations using eight-band k · pmodels and calculating intraband dipole matrix elementsreveal that for QDs, the term Eq. 6(b) is much larger(about an order of magnitude) than the term (a) calcu-lated from the envelopes involved; cf. Refs. [32, 34]. As aconsequence, the envelope part is neglected by previousinvestigations of single QDs and QD molecules (see Refs.[34, 35]), where an approximation for the dipole moment,which contains the central-cell term solely, is used; see,e.g., Ref. [33]. In agreement with previous investigations,we find for the QD series investigated that the transitiondipole moment calculated via term Eq. 6(b) is larger (byabout a factor of three to four) than the dipole momentcalculated from (a); see Fig. 4. As such our calculationsdemonstrate that term (a) has a not negligible impact onthe polarization of the CB intraband transitions; there-fore, the whole dipole moment is considered within oursimulations of the radiation anisotropy via Eq. 9.

4

Figure 3. Diagrams are calculated including effects of strain and strain-induced internal fields. (a) Decomposition of the lowestconduction band (CB) state of the cubodial QD series A into the |cb〉 (blue circles), |hh〉 (green empty square), |lh〉 (greenfilled square), and |so〉 (red pyramid) basis functions versus vertical aspect ratio (AR). (b) A plot of the energies for the threecorresponding Kramers-degenerate electron states, i.e., the px,y- (semi-filled circles) and s-type orbitals (filled circles), wheres-type state refers to | |ψs〉 |2, likewise for the excited states. The right y-axis shows the hydrostatic strain expectation valuefor the lowest CB state (orange diamonds), i.e., εh = 〈ψ1|εh|ψ1〉. (c and d) Plots of the conduction band edge VCB (black) andthe hydrostatic strain εh (orange) for the cubodial QDs with AR = 1.6 (c) and with AR = 0.4 (d).

A. The role of aspect ratio.

With the help of the series of artificial cubic QDs, weshow that the geometry of the confinement region alonechanges the radiation pattern. Therefore, we calculatedseries A without and with strain. Figure 2(a) shows thedifferent contributions of the VB functions |hh〉, |lh〉, and|so〉 to the lowest CB state without strain. Changing theQDs AR results in altering contributions of |hh〉 and |lh〉for AR > 1 and AR < 1 , while the |so〉 contributionremains more or less constant. In contrast to interbandtransitions, the atomic-like basis functions |x〉, |y〉, and|z〉 in Fig. 2(b) do not reflect the prevalent confinementregion, but as expected, the |x, y〉 and |z〉 fractions aredegenerate at AR = 1. The contribution of the |z〉 ba-sis function decreases with growing AR, while the |x, y〉contribution slightly decreases. In this regard, intrabandtransitions show a different characteristic compared tointerband transitions.Including strain and strain induced fields, the findings arevery similar; see Fig. 3(a). Here, also an enhancement ofthe |hh〉 and a reduction of the |lh〉 contribution withincreasing AR is observed. As discussed in Sec. II, theincreasing |hh〉-contribution results in an enhanced in-plane polarization, whereas, on the other hand, a larger|lh〉-contribution also raises the polarization within thegrowth direction z. Within the region of confinement, theCB edge shifts to higher energies the larger the hydro-static strain, and again, the hydrostatic strain becomesstronger the larger the region of confinement; see Figs.3(c,d) as well as Refs. [22, 65] for QD stacks. As a result,the contribution of the VB functions to the lowest CBstate is reduced and, likewise, its leading contribution,|cb〉-like, is increased. Similarly, an increasing AR re-duces the conduction-band-valence-band mixing; see Fig.3(a). The shift of the CB edge and the hydrostatic strainas a function of aspect ratio is also reflected in the evolu-tion of the energy eigenvalues of the first three Kramers-

0.511.520304050607080

vertical AR

relative

share[%

](a) (b)

(a)

0.511.5−0.4

−0.2

0

0.2

vertical aspect ratio

DORA

(110) (a) (b)

0.511.51

1.5

2

2.5

composition[%

]

(b)

Figure 4. (a) Relative share of the term (a) (blue pyra-mid) and term (b) (red inverted pyramid) contributing to thetransition dipole moment in Eq. 7 for the cubodial QD se-ries A versus aspect ratio. (b) DORA(110) of the term (a)(blue pyramid) and (b) (red inverted pyramid) in Eq. 7, re-spectively. The green axis depicts the contribution of the|hh〉 (green empty square) and |lh〉 (green filled square) basisfunctions from Fig. 3(a).

degenerate CB states; see Fig. 3(b). The p-to-s transitionenergies shift blue with increasing AR, raising the tran-sition matrix element Eq. 6. The hydrostatic strain ex-pectation value for the lowest CB state εh = 〈ψ1|εh|ψ1〉is increasing with AR reflecting the decreasing energyeigenvalues of the CB states.Figure 4(a) shows the relative shares of the transitiondipole moments in Eq. 7(a) versus (b) in the total dipolemoment for the py-to-s transitions of QDs in series A. Asthe AR increases, term (b) gains slightly over (a), with2.9 times greater than (a) for an AR = 1.6. Figure 4(b)shows the in-plane radiation DORA(110) determined viaEq. 11 for the terms (a) and (b), respectively. Also, thechange in the |hh〉 and |lh〉 components of the lowest CBstate from Fig. 3(a) is shown to illustrate the change interm (b) from nearly isotropic radiation for AR < 1.0to a radiation pattern perpendicular to (001)-plane forAR > 1.0. Term (a), in contrast, remains constant ata value of DORA(110) = −0.34, caused, as expected,by a strong anisotropic in-plane dipole moment of the

5

(a) (k)(f)

(b) (l)(g)

(c) (m)(h)

(d) (n)(i)

(e) (o)(j)

Figure 5. (a–e, k–o) normalized radiated power (Prad) persolid angle of the first and last QD structures within seriesA, B, and C, respectively. Blue and red radiation patternscorrespond to DORA(110) and DORA(110), respectively. (f–j) DORA(110) (blue semi-filled circle) and DORA(110) (redsemi-filled circle) of all QD structures investigated. As thesymmetry axis of the p-type are perpendicular to each other,the blue and red semi-filled circles correspond also to py- andpx-type CB states, respectively.

p-to-s transitions. This changes only minimally for anAR = 1.0, which is caused by the distinct shape of theinvolved orbitals for the artificial cubic QD at symmet-ric spatial confinement. Term (b) alone thus reflects thechange in the QD confinement region, resulting in en-hanced radiation perpendicular to the growth plane forQDs with AR > 1.0.The combined impact of terms (a) and (b) on the emis-sion directionality of series A is depicted in Figs. 5(a,f,k),

which results in a slightly more pronounced DORA ofDORA(110) & −46% for a AR > 1.0 compared to the in-dividual contributions of terms (a) and (b) shown in Fig.4(b). Figure 5(a) shows the radiation pattern within the(110)-plane at an AR = 1.6, which is highly anisotropicresulting from a strong in-plane polarization for the py-to-s transition. Compared to interband transitions (seeRef. [22] for AR < 1.0), intraband transitions at anAR > 1.0 result in a slightly more pronounced top emis-sion, which makes the contribution of the term (a) in Eq.7 apparent. For aspect ratios AR < 1.0, DORA is in-creasing, reflecting the growing |lh〉 contribution to thelowest CB state, but still making top emission more ef-fective than in-plane due to the term Eq. 7(a); see Fig.5(k). In Figure 6 (series A), the absolute values of thebasis functions |cb〉, |hh〉, |lh〉, and |so〉 orbitals are shownfor the vertical aspect ratios AR = 1.6, AR = 1.0, andAR = 0.4 in the (001)-plane. Here, |cb〉 is the sum of |cb1〉and |cb2〉, likewise for the other three basis functions. Forall ARs, the |hh〉-contribution exhibits a 4-fold symmetrywith a central node, resulting in a significant overlap withthe CB p-type orbitals. The |lh〉-contribution changes itssymmetry slightly from s-like for ARs < 1.0 to a mixtureof a 4-fold and s-like symmetry for ARs ≥ 1.0 withouta central node. Despite the |so〉-contribution is barelyinfluenced by changing the AR (cf. Figs. 2(a) and 3(a)),its symmetry changes from an s-like to a 4-fold symme-try with a central node for aspect rations AR < 1.0 and≥ 1.0, respectively. Due to the change in symmetry of the|so〉 basis function, the overlap with the p-type orbitalsincreases with aspect ratio, albeit not as pronounced asfor the |hh〉 function.

B. The role of number of stacked QDs.

In the second series we investigate the emission direc-tionality versus the number of stacked dots. We choosea barrier width of b = 0 for this series, as it representsthe maximal interdot coupling. Similarly, by omittingthe barrier, the influence of the AR on the emission pat-tern can be analyzed, also allowing a direct comparisonwith series A. Furthermore, experimental findings sug-gest that columnar QDs may stay in contact with eachother, if they were grown with a barrier of a few MLs[24–26].Figures 5(g,h) show the DORA values within the (110)-and (110)-plane for the py-to-s and px-to-s transitions,respectively. Beginning with a stack of four QDs, theemission directionality changes with further stackingfrom nearly isotropic for the single QD with DORA ≈−2% to a strong top emission with DORA > −36%.The change from an isotropic to a strongly anisotropicemission direction thus reflects the changing contribu-tions of the VB functions, with the |lh〉 contributionchanging to a predominant |hh〉 contribution for a stackof four QDs. We define a collective vertical aspectratio via the number of stacked QDs, ARcol(nQD) =

6

series: |cb〉 |hh〉 |lh〉 |so〉

A: AR = 1.6

C: b = 0ML

B: # = 10

A: AR = 1.0

A: AR = 0.4

B: # = 4

B: # = 1

C: b = 8ML

C: b = 16ML

Figure 6. The absolute values of the lowest conduction bandstate basis envelopes |cb〉, |hh〉, |lh〉, and |so〉 for three selectedgeometries of series A, B, and C in the (001)-plane integratedalong the [001]-axis and normalized to the maximum in eachsubfigure. Structures not shown resemble the symmetries ofthe envelopes depicted, e.g., AR = 1.6 resembles the symme-tries for aspect ratios larger than 1.0 and AR = 0.4 for ARssmaller than 1.0.

nQDhQD/(average QD width), which allows us to com-pare the ARcol with the AR from series A. As for series A,the emission directionality can be tuned to a strong topemission by stacking QDs to ARcol(nQD) ≥ 1.0; for ourseries B, the aspect ratio for four QDs is ARcol(4) = 0.92.Figures 5(b,c) and (l,m) depict the corresponding emis-sion patterns for a stack of ten QDs and a single QD,respectively, showing a strong top emission for stackswith nQD ≥ 4. Figures 5(g,h) also depict the DORAvalues for radiation parallel to the axis of the py and px-type orbitals, respectively, showing an isotropic radiationpattern, becoming slightly anisotropic for stacks of QDs

smaller than four. The symmetries of the VB functionsfor series B in Fig. 6 follow the same pattern as for seriesA.

C. The role of interdot separation.

With help of the last series C, we investigate the im-pact of increasing the interdot barrier b on the emissiondirectionality of stacked QDs. If QDs are stacked closelywith b = 0 MLs, a strong top emission with DORA val-ues of ≈ −40% are observed for a stack of five QDs; cf.Fig. 5(i,j). Figures 5(d,e) and (n,o) depict the radiationpattern for b = 0 MLs and b = 16 MLs, respectively.By increasing the interdot separation, the |hh〉- and |lh〉contributions shift towards the single QD case of SeriesB, or AR = 0.4 for series A. As shown in Ref. [22], theband structure and strain distribution is almost identi-cal to an uncoupled single QD. In contrast to series B,the emission directionality changes linearly from a strongtop to a more isotropic emission of DORA ≈ −15% and≈ 4%, respectively; cf. Fig. 5(i,j). The envelopes in Fig.6 show identical symmetries as for series B, despite the|so〉-contribution at b = 8 MLs showing a state changingfrom an s-like to a 4-fold symmetry. We note, however,that an anti-binding s-type state forms as the QDs sep-aration is increased, which would make measuring theradiation characteristics of the p-s transitions even moredifficult for stacks with large barriers; cf. Refs. [65].

IV. CONCLUSION

We demonstrate that the vertical emission of intra-band transitions of stacked QDs can be tuned via thestructure’s vertical aspect ratio. With the help of anartificial cuboidal QD, we show that the minor contri-butions from the central-cell part within the momentummatrix element change with aspect ratio enhancing orweakening the emission anisotropy. In contrast to inter-band transitions, the strain has a subordinate role andthe change of the aspect ratio itself results in a moredominant |lh〉/|hh〉 contribution of the lowest CB state.In addition, we find that the matrix elements amongthe envelope functions have a significant contribution tothe emission direction of stacked QDs and cannot be ne-glected.We investigate two series of QDs, investigating the im-pact of (i) the number of stacked QDs on the radiationpattern and (ii) the coupling strength between stackedQDs. Here we show that the results for the artificialQD can be transferred to realistic QD structures. In QDstacks, stacking QDs leads to a larger aspect ratio, thusenhancing the top emission for the CB intraband transi-tion, although this is only beneficial up to the isotropicwith an AR of 1.0, as further stacking then provides noadditional enhancement. Moreover, we show that thevertical emission is enhanced with increasing AR, vice

7

versa to the interband transitions in QDs. By increasingthe interdot distance in QD stacks, i.e., weakening theQD coupling strength, the emission pattern converges toa single QD, reducing the vertical emission to a moreisotropic pattern.Similar to interband transitions, our calculations showqualitative changes in the radiation pattern of QD stacksand provide qualitative values of the degree of radiationanisotropy (DORA) for the parameters considered. Inaddition, we provide insight into the contribution of theenvelope functions versus the central cell fraction to theemission rate and pattern. Our calculations also considerthe contribution of the envelope functions to the emission

pattern, which has been neglected in previous studiesof the polarization of intraband transitions as its con-tribution is comparatively small. Therefore, our studiesprovide new insight into the radiation anisotropy of QDintraband transitions, especially for stacked QDs, whichmay be beneficial for designing future infrared deviceswith enhanced in-plane or top emission polarization.

ACKNOWLEDGMENTS

The authors would like to thank Dirk Ziemann forreading the manuscript and for the fruitful and construc-tive discussions.

[1] T. Nagatsuma, G. Ducournau, and C. C. Renaud, Ad-vances in terahertz communications accelerated by pho-tonics, Nature Photonics 10, 371 (2016).

[2] A. Khalatpour, A. K. Paulsen, C. Deimert, Z. R.Wasilewski, and Q. Hu, High-power portable terahertzlaser systems, Nature Photonics 15, 16 (2021).

[3] H. Sarieddeen, N. Saeed, T. Y. Al-Naffouri, and M.-S.Alouini, Next Generation Terahertz Communications: ARendezvous of Sensing, Imaging, and Localization, IEEECommunications Magazine 58, 69 (2020).

[4] M. Koch, Terahertz Communications: A 2020 vision, inTerahertz Frequency Detection and Identification of Ma-terials and Objects, edited by R. E. Miles, X.-C. Zhang,H. Eisele, and A. Krotkus (Springer Netherlands, Dor-drecht, 2007) pp. 325–338, series Title: NATO Sciencefor Peace and Security Series.

[5] M. Tonouchi, Cutting-edge terahertz technology, NaturePhotonics 1, 97 (2007).

[6] D. Bimberg, M. Grundmann, and N. N. Ledentsov,Quantum dot heterostructures (John Wiley & Sons,1999).

[7] N. Kirstaedter, N. Ledentsov, M. Grundmann, D. Bim-berg, V. Ustinov, S. Ruvimov, M. Maximov, P. S. Kop’ev,Z. I. Alferov, U. Richter, et al., Low threshold, large t/subo/injection laser emission from (inga) as quantum dots,Electronics Letters 30, 1416 (1994).

[8] Y. Arakawa and H. Sakaki, Multidimensional quantumwell laser and temperature dependence of its thresholdcurrent, Applied physics letters 40, 939 (1982).

[9] M. Grundmann, J. Christen, N. Ledentsov, J. Bohrer,D. Bimberg, S. Ruvimov, P. Werner, U. Richter,U. Gosele, J. Heydenreich, et al., Ultranarrow lumines-cence lines from single quantum dots, Physical ReviewLetters 74, 4043 (1995).

[10] X. Tang, M. M. Ackerman, M. Chen, and P. Guyot-Sionnest, Dual-band infrared imaging using stacked col-loidal quantum dot photodiodes, Nature Photonics 13,277 (2019).

[11] T. Murata, S. Asahi, S. Sanguinetti, and T. Kita, In-frared photodetector sensitized by inas quantum dots em-bedded near an al 0.3 ga 0.7 as/gaas heterointerface, Sci-entific Reports 10, 1 (2020).

[12] E.-T. Kim, A. Madhukar, Z. Ye, and J. C. Campbell,High detectivity inas quantum dot infrared photodetec-

tors, Applied Physics Letters 84, 3277 (2004).[13] D. Pan, E. Towe, and S. Kennerly, Normal-incidence in-

tersubband (in, ga) as/gaas quantum dot infrared pho-todetectors, Applied Physics Letters 73, 1937 (1998).

[14] M. Nagashima, M. Kibe, M. Doshida, Y. Uchiyama,Y. Matsukura, and H. Nishino, Photodetection around 10µ m wavelength using s-p transitions in inas/alas/algaasself-assembled quantum dots, Journal of Applied Physics107, 054504 (2010).

[15] J. C. Campbell and A. Madhukar, Quantum-dot in-frared photodetectors, Proceedings of the IEEE 95, 1815(2007).

[16] A. Mittelstadt, L. A. T. Greif, S. T. Jagsch, andA. Schliwa, Terahertz lasing at room temperature: Anumerical study of a vertical-emitting quantum cascadelaser based on a quantum dot superlattice, Physical Re-view B 103, 115301 (2021).

[17] I. A. Dmitriev and R. A. Suris, Quantum cascade lasersbased on quantum dot superlattice, physica status solidi(a) 202, 987 (2005).

[18] M. C. Beard, A. G. Midgett, M. C. Hanna, J. M. Luther,B. K. Hughes, and A. J. Nozik, Comparing multiple ex-citon generation in quantum dots to impact ionizationin bulk semiconductors: implications for enhancement ofsolar energy conversion, Nano letters 10, 3019 (2010).

[19] K. A. Sablon, J. W. Little, V. Mitin, A. Sergeev, N. Vagi-dov, and K. Reinhardt, Strong enhancement of solar cellefficiency due to quantum dots with built-in charge, Nanoletters 11, 2311 (2011).

[20] A. Barve and S. Krishna, Photovoltaic quantumdot quantum cascade infrared photodetector, AppliedPhysics Letters 100, 021105 (2012).

[21] T. Sugaya, O. Numakami, S. Furue, H. Komaki,T. Amano, K. Komori, K. Matsubara, Y. Okano, andS. Niki, Ultra-high stacks of InGaAs quantum dots forhigh efficiency solar cells, in 2011 37th IEEE PhotovoltaicSpecialists Conference (IEEE, Seattle, WA, USA, 2011)pp. 002661–002664.

[22] L. A. T. Greif, S. T. Jagsch, M. R. Wagner, andA. Schliwa, Tuning the Emission Directionality ofStacked Quantum Dots, ACS Photonics 5, 4838 (2018).

[23] P. Yu, W. Langbein, K. Leosson, J. M. Hvam,N. Ledentsov, D. Bimberg, V. Ustinov, A. Y. Egorov,A. Zhukov, A. Tsatsul’nikov, et al., Optical anisotropy

8

in vertically coupled quantum dots, Physical Review B60, 16680 (1999).

[24] T. Kita, O. Wada, H. Ebe, Y. Nakata, andM. Sugawara, Polarization-independent photolumines-cence from columnar inas/gaas self-assembled quantumdots, Japanese journal of applied physics 41, L1143(2002).

[25] T. Kita, P. Jayavel, O. Wada, H. Ebe, Y. Nakata, andM. Sugawara, Polarization controlled edge emission fromcolumnar inas/gaas self-assembled quantum dots, phys-ica status solidi (c) , 1137 (2003).

[26] T. Kita, N. Tamura, O. Wada, M. Sugawara, Y. Nakata,H. Ebe, and Y. Arakawa, Artificial control of opticalgain polarization by stacking quantum dot layers, Ap-plied physics letters 88, 211106 (2006).

[27] P. Ridha, L. Li, M. Rossetti, G. Patriarche, and A. Fiore,Polarization dependence of electroluminescence fromclosely-stacked and columnar quantum dots, Optical andQuantum Electronics 40, 239 (2008).

[28] Y. Ikeuchi, T. Inoue, M. Asada, Y. Harada, T. Kita,E. Taguchi, and H. Yasuda, Multidirectional observationof photoluminescence polarization anisotropy in closelystacked inas/gaas quantum dots, Applied physics express4, 062001 (2011).

[29] N. Yasuoka, H. Ebe, K. Kawaguchi, M. Ekawa,S. Sekiguchi, K. Morito, O. Wada, M. Sugawara,and Y. Arakawa, Polarization-insensitive quantum dotsemiconductor optical amplifiers using strain-controlledcolumnar quantum dots, Journal of lightwave technology30, 68 (2011).

[30] M. Usman, T. Inoue, Y. Harda, G. Klimeck, and T. Kita,Experimental and atomistic theoretical study of degreeof polarization from multilayer InAs/GaAs quantum dotstacks, Physical Review B 84, 115321 (2011).

[31] M. Usman, Atomistic theoretical study of electronic andpolarization properties of single and vertically stacked el-liptical inas quantum dots, Physical Review B 86, 155444(2012).

[32] H. Jiang and J. Singh, Self-assembled semiconductorstructures: Electronic and optoelectronic properties,IEEE journal of quantum electronics 34, 1188 (1998).

[33] O. Stier, M. Grundmann, and D. Bimberg, Electronicand optical properties of strained quantum dots modeledby 8-band k·p theory, Physical Review B 59, 5688 (1999).

[34] W. Sheng and J.-P. Leburton, Enhanced intraband tran-sitions with strong electric-field asymmetry in stackedinas/gaas self-assembled quantum dots, Physical ReviewB 64, 153302 (2001).

[35] W. Sheng, Polarization of intersubband transitions inself-assembled quantum dots, Applied Physics Letters92, 043113 (2008).

[36] A. Adawi, E. Zibik, L. Wilson, A. Lemaitre, J. Cock-burn, M. Skolnick, M. Hopkinson, G. Hill, S. Liew, andA. Cullis, Strong in-plane polarized intraband absorptionin vertically aligned ingaas/gaas quantum dots, Appliedphysics letters 82, 3415 (2003).

[37] B. Carpenter, E. Zibik, M. Sadowski, L. Wilson, D. Whit-taker, J. Cockburn, M. Skolnick, M. Potemski, M. Steer,and M. Hopkinson, Intraband magnetospectroscopy ofsingly and doubly charged n-type self-assembled quan-tum dots, Physical Review B 74, 161302 (2006).

[38] J. He, H. J. Krenner, C. Pryor, J. Zhang, Y. Wu,D. Allen, C. Morris, M. Sherwin, and P. M. Petroff,Growth, structural, and optical properties of self-

assembled (in, ga) as quantum posts on gaas, Nano letters7, 802 (2007).

[39] T. Saito, H. Ebe, Y. Arakawa, T. Kakitsuka, and M. Sug-awara, Optical polarization in columnar InAs/GaAsquantum dots: 8-band k·p calculations, Physical ReviewB 77, 195318 (2008).

[40] P. Ridha, L. H. Li, M. Mexis, P. M. Smowton, J. An-drzejewski, G. Sek, J. Misiewicz, E. P. O’Reilly, G. Patri-arche, and A. Fiore, Polarization properties of columnarquantum dots: effects of aspect ratio and compositionalcontrast, IEEE journal of quantum electronics 46, 197(2009).

[41] M. Usman, In-plane polarization anisotropy of groundstate optical intensity in inas/gaas quantum dots, Jour-nal of Applied Physics 110, 094512 (2011).

[42] X. Yuan, F. Weyhausen-Brinkmann, J. Martın-Sanchez,G. Piredda, V. Krapek, Y. Huo, H. Huang, C. Schimpf,O. G. Schmidt, J. Edlinger, et al., Uniaxial stress flips thenatural quantization axis of a quantum dot for integratedquantum photonics, Nature communications 9, 1 (2018).

[43] T. Sugaya, Y. Kamikawa, S. Furue, T. Amano, M. Mori,and S. Niki, Multi-stacked quantum dot solar cells fabri-cated by intermittent deposition of InGaAs, Solar EnergyMaterials and Solar Cells 95, 163 (2011).

[44] L. Li, P. Ridha, G. Patriarche, N. Chauvin, and A. Fiore,Shape-engineered epitaxial ingaas quantum rods for laserapplications, Applied Physics Letters 92, 121102 (2008).

[45] H. Blank, D. Litvinov, R. Schneider, D. Gerthsen, T. Pas-sow, and K. Scheerschmidt, Quantification of the In-distribution in embedded InGaAs quantum dots by trans-mission electron microscopy, Crystal Research and Tech-nology 44, 1083 (2009).

[46] D. Litvinov, H. Blank, R. Schneider, D. Gerthsen,T. Vallaitis, J. Leuthold, T. Passow, A. Grau, H. Kalt,C. Klingshirn, and M. Hetterich, Influence of InGaAs caplayers with different In concentration on the properties ofInGaAs quantum dots, Journal of Applied Physics 103,083532 (2008).

[47] T. Inoue, M. Asada, N. Yasuoka, O. Kojima, T. Kita,and O. Wada, Polarization control of electroluminescencefrom vertically stacked inas/gaas quantum dots, AppliedPhysics Letters 96, 211906 (2010).

[48] T. Kita, N. Tamura, O. Wada, M. Sugawara, Y. Nakata,H. Ebe, and Y. Arakawa, Artificial control of opticalgain polarization by stacking quantum dot layers, Ap-plied Physics Letters 88, 211106 (2006).

[49] D. M. Bruls, J. W. A. M. Vugs, P. M. Koenraad,H. W. M. Salemink, J. H. Wolter, M. Hopkinson, M. S.Skolnick, F. Long, and S. P. A. Gill, Determination of theshape and indium distribution of low-growth-rate inasquantum dots by cross-sectional scanning tunneling mi-croscopy, Applied Physics Letters 81, 1708 (2002).

[50] A. Lemaıtre, G. Patriarche, and F. Glas, Compositionprofiling of InAs/GaAs quantum dots, Applied PhysicsLetters 85, 3717 (2004).

[51] P. W. Fry, I. E. Itskevich, D. J. Mowbray, M. S. Skol-nick, J. J. Finley, J. A. Barker, E. P. O’Reilly, L. R.Wilson, I. A. Larkin, P. A. Maksym, M. Hopkinson,M. Al-Khafaji, J. P. R. David, A. G. Cullis, G. Hill, andJ. C. Clark, Inverted electron-hole alignment in inas-gaasself-assembled quantum dots, Phys. Rev. Lett. 84, 733(2000).

[52] J. A. Barker and E. P. O’Reilly, Theoretical analysis ofelectron-hole alignment in inas-gaas quantum dots, Phys.

9

Rev. B 61, 13840 (2000).[53] M. Sabathil, S. Hackenbuchner, S. Birner, J. Majewski,

P. Vogl, and J. Finley, Theory of vertical and lateral starkshifts of excitons in quantum dots, physica status solidi(c) , 1181 (2003).

[54] M. Usman, V. Tasco, M. T. Todaro, M. De Giorgi, E. P.O’Reilly, G. Klimeck, and A. Passaseo, The polariza-tion response in inas quantum dots: theoretical correla-tion between composition and electronic properties, Nan-otechnology 23, 165202 (2012).

[55] M. Grundmann, O. Stier, and D. Bimberg, InAs/GaAspyramidal quantum dots: Strain distribution, opticalphonons, and electronic structure, Physical Review B 52,11969 (1995).

[56] A. Schliwa, M. Winkelnkemper, and D. Bimberg, Impactof size, shape, and composition on piezoelectric effectsand electronic properties of In(Ga)As/GaAs quantumdots, Physical Review B 76, 205324 (2007).

[57] G. Bester, X. Wu, D. Vanderbilt, and A. Zunger, Im-portance of Second-Order Piezoelectric Effects in Zinc-Blende Semiconductors, Physical Review Letters 96(2006).

[58] G. Bester, A. Zunger, X. Wu, and D. Vanderbilt, Effectsof linear and nonlinear piezoelectricity on the electronic

properties of InAs/GaAs quantum dots, Physical ReviewB 74 (2006).

[59] O. Stier and D. Bimberg, Modeling of strained quantumwires using eight-band k·p theory, Physical Review B 55,7726 (1997).

[60] O. Stier, Electronic and Optical Properties of QuantumDots and Wires (Wissenschaft & Technik Verlag, 2000).

[61] S. L. Chuang, Efficient band-structure calculations ofstrained quantum wells, Physical Review B 43, 9649(1991).

[62] P. Enders, A. Barwolff, M. Woerner, and D. Suisky, k·ptheory of energy bands, wave functions, and optical selec-tion rules in strained tetrahedral semiconductors, Phys.Rev. B 51, 16695 (1995).

[63] S. L. Chuang, Physics of Optoelectronic Devices, 2nd ed.,Wiley series in pure and applied optics (John Wiley &Sons, Hoboken, N.J, 2009).

[64] I. Vurgaftman, J. R. Meyer, and L. R. Ram-Mohan, Bandparameters for III-V compound semiconductors and theiralloys, Journal of Applied Physics 89, 5815 (2001).

[65] A. Mittelstadt, L. A. T. Greif, S. T. Jagsch, andA. Schliwa, Efficient electronic structure calculations forextended systems of coupled quantum dots using a linearcombination of quantum dot orbitals method, PhysicalReview B 103, 115302 (2021).